Synthesis of hexagonal boron nitride
Two dimensional hexagonal boron nitride (2D h-BN) is a material of comparable structure to graphene with potential applications in e.g. photonics., fuel cells  and as a substrate for two-dimensional heterostructures. 2D h-BN is isostructural to graphene, but where graphene is conductive, 2D h-BN is a wide-gap insulator.
The properties of 2D h-BN films depends greatly on the quality of the films. It has been challenging to synthesize high-quality 2D h-BN over large areas. In particular, the small grain size of polycrystalline h-BN results in many grain boundaries, which create charge traps and higher surface roughness.
The production of 2D h-BN can be divided into top-down and bottom-up approaches. In bottom-up methods, a film is grown or deposited on a surface; in top-down methods, a larger structure is reduced until the desired state or structure is achieved.
The general idea behind top-down approaches is to take bulk h-BN, break the Van der Waals forces between the hexagonal layers and separate the resulting two-dimensional sheets of h-BN. These techniques mainly consist of mechanical and chemical exfoliation methods.
In mechanical exfoliation the atomic sheets of h-BN are physically pulled or separated from each other. For example using regular adhesive tape to peel off graphene sheets is one of the most famous mechanical exfoliation methods and similar techniques can also be used to create h-BN sheets. Generally speaking mechanical exfoliation methods can be considered as simple ways to fabricate h-BN nanosheets, but their yield can be small  and the size of the fabricated structures is usually limited. On the other hand, the number of defects on the produced nanosheets has been found to be smaller compared to chemical methods.
Chemical exfoliation is carried out in liquid solvents such as dichloroethane and dimethylformamide. Sonication is used to break Van der Waals forces in h-BN crystals which allows the solvent molecules to expand the atomic layers. These methods are quite simple and can also provide a higher yield compared to mechanical exfoliation, although the samples are easily contaminated.
Chemical Vapor DepositionEdit
Chemical Vapor Deposition (CVD) is a bottom-up chemical deposition method used to construct high-quality nanoscale films. In CVD, a substrate is exposed to precursors, which react on the wafer surface to produce the desired film. This reaction often also results in toxic byproducts. Historically, ultra-high vacuum CVD (UHVCVD) has been used for thin h-BN deposition on transition metals. More recently, CVD of h-BN has also been successful on metallic surfaces at higher pressures. 
CVD is reliant on the use of reactive precursors. For h-BN, there are gaseous, liquid, and solid options to choose from, each with their respective advantages and drawbacks. Gaseous precursors, such as BF3/NH3, BCl3/NH3, and B2H6/NH3, are toxic and require careful ratios of gases to preserve a 1:1 B/N stoichiometry. Liquid precursors, such as borazine, have equal amounts of boron and nitrogen, and do not produce highly toxic side products. However, they are sensitive to moisture, and hydrolyze readily. This drawback can be counteracted by raising the temperature, but higher temperatures also result in increased rates of reaction. Finally, for solid precursors, borazane is stable and has a 1:1 B/N stoichiometry. Its drawback is its decomposition into the highly active BH2NH2, which polymerizes at room temperature. Pure borazane consequently does not work as a precursors, and should be mixed with BH2NH2 and borazine.
CVD is classified by its operation conditions into atmospheric pressure CVD (APCVD), low-pressure CVD (LPCVD) and ultra-high vacuum CVD. Higher vacuums require more sophisticated equipment, and higher operation costs, while higher pressures yield faster growth. For h-BN, APCVD has been unable to precisely control the number of layers. At least LPCVD is currently required to produce large area monolayer h-BN.
The choice of substrate in CVD is important, as the film under production must stick to the surface. In h-BN, as in graphene, transition metals such as Cu or Ni are popular choices for CVD substrate materials. Platinum has also been used as a wafer, as has iron foil  and cobalt. The drawback with catalytic transition metal wafer materials is the need to transfer the end result to a target substrate, such as silicon. This procedure often damages or contaminates the film. Some h-BN films have been grown on Si, SiO2/Si, and sapphire 
The orientation of domains on the h-BN film is affected by the choice of substrate material and its orientation. Typically, domains are triangular in LPCVD, and triangular, truncated triangular, or hexagonal in APCVD. Often, these domains are randomly oriented, but h-BN domains align strictly with copper (100) or (111) surface lattices. With Cu (110), alignment is less strict, but still strong over millimeter distances.
Physical Vapor DepositionEdit
In sputtering, a solid target of the desired film material is bombarded with energetic particles, so that a thin film can be produced on a wafer facing the target. Ar ion beams have been used to sputter h-BN on Cu foils, resulting in high-quality, few-layer films, and magnetron sputtering of B in N2/Ar has been used to grow high-quality h-BN on Ru. This process results in films two atomic layers thick; thicker films can be grown by alternating room temperature deposition and annealing cycles.
When a source of boron and nitrogen, such as amorphous BN, is sandwiched between a Co or Ni film and SiO2, it is possible to grow an atomically thin h-BN film on the metal surface by annealing the heterostructure in a vacuum. The B and N atoms dissolve in the metal bulk, diffuse through the film, and precipitate on the surface. In this way, the use of unconventional or toxic precursors is avoided.
Molten boron oxide reacts with gaseous ammonia to form an ultrathin h-BN film at the reaction interface. The film grows to 20-30 nm in thickness, after which the process self-terminates, the setup is cooled down, and the boron oxide can be dissolved in water.
- Andres Castellanos-Gomez (2016). "Why all the fuss about 2D semiconductors?". Nature Photonics. 10 (4): 202–204. arXiv:1604.06425. Bibcode:2016NaPho..10..202C. doi:10.1038/nphoton.2016.53.
- Hu, S.; et al. (2014). "Proton transport through one-atom-thick crystals". Nature. 516 (7530): 227–230. arXiv:1410.8724. Bibcode:2014Natur.516..227H. doi:10.1038/nature14015.
- Wang, H.; et al. (2017). "Recent progress in synthesis of two-dimensional hexagonal boron nitride". Journal of Semiconductors. 38 (3): 031003. Bibcode:2017JSemi..38c1003W. doi:10.1088/1674-4926/38/3/031003.
- Novoselov K. S.; et al. (2004). "Electric field effect in atomically thin carbon films". Science. 306 (5696): 666–669. arXiv:cond-mat/0410550. Bibcode:2004Sci...306..666N. doi:10.1126/science.1102896.
- Novoselov K. S.; et al. (2005). "Two-dimensional atomic crystals". Proc Natl Acad Sci USA. 102 (30): 10451–10453. arXiv:cond-mat/0503533. Bibcode:2005PNAS..10210451N. doi:10.1073/pnas.0502848102.
- Xu M. S.; et al. (2013). "Graphene-like two-dimensional materials". Chem. Rev. 113 (5): 3766–3798. doi:10.1021/cr300263a.
- Bao, Jie; et al. (2016). "Synthesis and applications of two-dimensional hexagonal boron nitride in electronics manufacturing". Electronic Materials Letters. 12 (1): 1–16. Bibcode:2016EML....12....1B. doi:10.1007/s13391-015-5308-2.
- Warner J. H.; et al. (2010). "Atomic resolution imaging and topography of boron nitride sheets produced by chemical exfoliation". ACS Nano. 4 (3): 1299–1304. doi:10.1021/nn901648q.
- Zhi C.; et al. (2009). "Large-scale fabrication of few-atomic-layer boron nitride nanosheets and their utilization in polymeric composites with improved thermal and mechanical properties". Adv. Mater. 21 (28): 2889–2893. doi:10.1002/adma.200900323.
- Nagashima, A.; et al. (1995). "Electronic structure of monolayer hexagonal boron nitride physisorbed on metal surfaces". Physical Review Letters. 75 (21): 3918–3921. Bibcode:1995PhRvL..75.3918N. doi:10.1103/PhysRevLett.75.3918. PMID 10059764.
- Kim, G.; et al. (2013). "Growth of high-crystalline, single-layer hexagonal boron nitride on recyclable platinum foil". Nano Letters. 13 (4): 1834–1839. Bibcode:2013NanoL..13.1834K. doi:10.1021/nl400559s.
- Pierson, Hugh O. (1975). "Boron Nitride Composites By Chemical Vapor Deposition". Journal of Composite Materials. 9 (3): 228–240.
- Sun, Yongzhou; et al. (2015). "Behavior of decomposed ammonia borane at high pressure". Journal of Physics and Chemistry of Solids. 84: 75–79. Bibcode:2015JPCS...84...75S. doi:10.1016/j.jpcs.2014.12.004.
- Koepke, Justic C.; et al. (2016). "Role of Pressure in the Growth of Hexagonal Boron Nitride Thin Films from Ammonia-Borane". Chemistry of Materials. 28 (2): 4169–4179. arXiv:1605.06861. doi:10.1021/acs.chemmater.6b00396.
- Gao, Yang; et al. (2013). "Repeated and Controlled Growth of Monolayer, Bilayer and Few-Layer Hexagonal Boron Nitride on Pt Foils". ACS Nano. 7 (6): 5199–5206. doi:10.1021/nn4009356.
- Kim SM; et al. (2015). "Synthesis of large-area multilayer hexagonal boron nitride for high material performance". Nature Communications. 6. Bibcode:2015NatCo...6E8662K. doi:10.1038/ncomms9662. PMC 4639899.
- Orofeo, Carlo M.; et al. (2013). "Growth and low-energy electron microscopy characterization of monolayer hexagonal boron nitride on epitaxial cobalt". Nano Research. 6 (5): 335–347. doi:10.1007/s12274-013-0310-1.
- Yu, Jie; et al. (2010). "Vertically Aligned Boron Nitride Nanosheets: Chemical Vapor Synthesis, Ultraviolet Light Emission, and Superhydrophobicity". ACS Nano. 4 (1): 414–422. doi:10.1021/nn901204c.
- Jang, A-Rang; et al. (2016). "Wafer-Scale and Wrinkle-Free Epitaxial Growth of Single-Orientated Multilayer Hexagonal Boron Nitride on Sapphire". Nano Letters. 16 (5): 3360–3366. Bibcode:2016NanoL..16.3360J. doi:10.1021/acs.nanolett.6b01051.
- Liu, Lei; et al. (2014). "Unusual role of epilayer–substrate interactions in determining orientational relations in van der Waals epitaxy". Proc Natl Acad Sci USA. 111 (47): 16670–16675. Bibcode:2014PNAS..11116670L. doi:10.1073/pnas.1405613111. PMC 4250159.
- Tay, Roland Yingjie; et al. (2016). "Synthesis of aligned symmetrical multifaceted monolayer hexagonal boron nitride single crystals on resolidified copper". Nanoscale. 8 (4): 2434–2444. Bibcode:2016Nanos...8.2434T. doi:10.1039/C5NR08036C.
- Wang, H.; et al. (2015). "Controlled Growth of Few‐Layer Hexagonal Boron Nitride on Copper Foils Using Ion Beam Sputtering Deposition". Small. 11 (13): 1542–1547. doi:10.1002/smll.201402468.
- Sutter, P.; et al. (2013). "Scalable Synthesis of Uniform Few-Layer Hexagonal Boron Nitride Dielectric Films". Nano Letters. 13 (1): 276–281. Bibcode:2013NanoL..13..276S. doi:10.1021/nl304080y.
- Suzuki, Satoru; et al. (2012). "Growth of atomically thin hexagonal boron nitride films by diffusion through a metal film and precipitation". J. Phys. D: Appl. Phys. 45 (38): 385304. Bibcode:2012JPhD...45L5304S. doi:10.1088/0022-3727/45/38/385304.
- Nakhaie, S.; et al. (2015). "Synthesis of atomically thin hexagonal boron nitride films on nickel foils by molecular beam epitaxy". Appl. Phys. Lett. 106 (21): 213108. arXiv:1501.06606. Bibcode:2015ApPhL.106u3108N. doi:10.1063/1.4921921.
- Yang, X.; et al. (2013). "Facile synthesis of large-area ultrathin hexagonal BN films via self-limiting growth at the molten B2O3 surface". Small. 9 (8): 1353. doi:10.1002/smll.201203126.